development of lightweight bulletproof vest inserts with yadda.icm.edu.pl/yadda/element/...
Post on 06-Jun-2020
Embed Size (px)
This paper is based on the work presented at the 10th International Armament Conference on „Scientific Aspects of Armament and Safety Technology”, Ryn, Poland, September 15-18, 2014.
Development of Lightweight Bulletproof Vest Inserts with
Increased Protection Capability
Marcin CEGŁA, Wiesław HABAJ, Paweł PODGÓRZAK*
Military Institute of Armament Technology, 7 Wyszyńskiego St., 05-220 Zielonka, Poland
* corresponding author, e-mail: firstname.lastname@example.org
Manuscript received May 27, 2014. Final manuscript received September 08, 2014 Abstract. The paper presents a problem of protection against modern pistol ammunition with increased armour-piercing capabilities. Traditional bulletproof vests made of polyethylene or aramid fiber-based fabrics give acceptable protection against lead-core pistol ammunition and fragments but they are insufficient for AP steel core penetration. In such case, the use of ceramic materials is essential. The article presents results of ballistic tests of composite material sets involving silicon carbide (SiC) and boron carbide (B4C) ceramics against 5.7 × 28 and 4.6 × 30 mm projectiles. Primary aspects of concealed bulletproof vest construction are also described. Keywords: ballistic protection, armour ceramics, concealed bulletproof vest 1. INTRODUCTION AND PREVIOUS WORK 1.1. Composition and role of the bulletproof vest
Lightweight bulletproof vests are commonly used among police, military
and government special forces.
PROBLEMS OF MECHATRONICS ARMAMENT, AVIATION, SAFETY ENGINEERING
ISSN 2081-5891 5, 3 (17), 2014, 23-34
M. Cegła, W. Habaj, P. Podgórzak 24
They give protection from most types of pistol ammunition and fragments as well as against larger threats like some carbine or rifle bullets . A modern bulletproof vest is a multilayered structure in which every layer has its role in stopping the projectile and reducing its effect on the body of the user. Main part of the vest are soft ballistic panels responsible for stopping less lethal threats as pistol ammunition, fragments, and in some cases blades and spikes. The best known soft fiber based materials are aramid fabrics Kevlar® or Twaron® and ultra-high-molecular weight polyethylene fibers Spectra® and Dyneema® . In case of protection against more lethal threats, ceramic hard plates are used as inserts for body armours. The most commonly used ceramic materials are alumina (Al2O3), silicon carbide (SiC), and boron carbide (B4C). Finally, special purpose layers can be added to the vest. Among them are trauma absorbing materials that spread kinetic energy transmitted from the projectile and which reduce backface deformation or stab resisting materials designed to defeat blades and spikes [1-3]. A typical multi-layered bulletproof vest construction is shown in Figure 1.
1. Vest outer cover, 2. Soft backing layer, 3. Hard ballistic insert outer
cover, 4. Inner ceramic carrier, 5. Adhesive layer, 6. Ceramic tile layer.
Fig. 1. Example of the bulletproof vest construction
A special group of light body armours are concealed bulletproof vests. A key requirement for these vests, which are worn under clothing, is functional deformation. This term refers to sufficient deformability for the intended applications. This definition can refer to ceramic-based ballistic inserts. As new types of ammunition with increased penetration capabilities appear on the market there is a demand for development of special concealed body armour which will combine excellent ballistic properties of advanced ceramic materials applied in zones, with ability to deform and adjust its shape to the body of the user. The vest must, at the same time, have the lowest possible weight.
Development of Lightweight Bulletproof Vest Inserts with Increased… 25
With the available materials, meeting all these requirements at the same time is a very difficult task as the total weight of the vest and its protective area are a function of type of ceramics used, the technology applied, and the construction of the whole armour system [1, 4]. 1.2. New protection requirements
Along with the development of individual bulletproof vests with increased protection characteristics, the introduction of modern pistol ammunition with increased penetration capabilities came. High velocities and small diameter of the projectiles together with armour piercing structure influence their high abilities to penetrate personal body armour. The possibility to be fired from relatively small hand guns and sub-machine guns makes additional threat for police, military, and special government forces. Among these threats, the most common are 5.7 × 28 mm SS190 projectiles developed by FN Herstal and 4.6 × 30 mm DM21 and DM31 projectiles developed by Heckler & Koch . Three mentioned types of ammunition will be used in further research therefore they will be described in detail. Table 1 presents construction and average velocities of these projectiles. The order shown in the table corresponds to the threat level that these projectiles possess to body armour.
Table 1. Modern pistol ammunition with increased penetration capability 
4.6 × 30 mm DM21
2.6 613 Lead core, full metal jacket
5.7 × 28 mm SS190
2 703 Brass jacket, aluminium core with steel penetrator in top
section 4.6 × 30 mm
DM31 2 687 Steel monoblock plated with
The DM21 projectile is a classic lead core, construction similar to traditional 9 × 19 mm Parabellum. Its advantage is relatively high velocity. Considerably dangerous is the SS190 due to hybrid structure of the projectile and the highest, among the others, average velocity. It can be qualified as projectile with increased penetration capability. The DM31, however, is a pure armour piercing projectile with a sharp steel monoblock core, which combined with high velocity makes it a serious threat for any personal body armour. Figure 2 presents the condition of projectiles after penetrating into composite sample made of ceramic front layer and soft fiber-based backing layer, as well as X-ray photographs of these samples. DM21 and SS190 projectiles were fired on the same sample while the DM31 required a thicker ceramic layer.
M. Cegła, W. Habaj, P. Podgórzak 26
DM21 SS190 DM31 e
DM21 SS190 DM31
Fig. 2. Projectiles after impact The DM21 was completely destroyed on the ceramic front layer and the elements of steel jacket and lead core were retrieved from the backing layer (Fig. 2a and 2e). The composite set design to protect against the SS190 projectile is more than enough for the DM21. The 5.7 × 28 mm projectile is most of the times divided in two separated pieces, the deformed aluminium core (Fig. 2b, 2f) and steel penetrator top (Fig. 2c). The DM31 steel projectile was blunted by the ceramic front (Fig. 2d) layer and rotated (Fig. 2g) allowing effective stopping by the backing layer. 1.3. Previous work
Table 2 presents preliminary results of firing tests of soft polyethylene and
aramid-based backings used in the construction of bulletproof vests with the use of 5.7 × 28 mm SS190 and 4.6 × 30 mm DM31 projectiles. The samples measured 400 × 400 mm and they were mounted on the base of clay. All ballistic tests were carried out in the ballistic tunnel at the temperature of 23.5°C, pressure of 995.6 hPa, and humidity of 38.96% RH.
Development of Lightweight Bulletproof Vest Inserts with Increased… 27
Table 2. Results of ballistic test for soft fiber-based fabrics [3, 4]
Projectile V0 [m/s]
[kg/m 2 ]
1 4.6 × 30 mm DM31
731 SB21 225 31.5 34 Perforation
2 4.6 × 30 mm DM31
718 GF4 225 52 45 Perforation
3 5.7 × 28 mm SS190
706 SB21 150 21 30 Perforation
4 5.7 × 28 mm SS190
702 SB21 150 21 30 Stopped at 135 layer
5 5.7 × 28 mm SS190
710 GF4 150 34.5 30 Perforation
6 5.7 × 28 mm SS190
705 GF4 180 41 36 Stopped at 170 layer
* SB21: non-woven fiber-based polyethylene Dyneema®,GF4: non-woven fiber-based aramid Goldflex®
The DM31 projectile penetrated the 225-layer material sets of Dyneema® and Goldflex® with no visible effect on the flight path. In similar experiment, the SS190 projectile was stopped with 150 layers of SB21 and 180 layers of GF4. These results exclude the application of material set made only of soft, fiber-based composites due to excessively high areal density and thickness. If the bulletproof vest is to maintain its concealed characteristics, another approach must be used. The idea of creating a lightweight bulletproof vest with increased protection capabilities involves right selection of ceramic segments, their individual bonding with the support layer and combining with deformable multi-layer, polyethylene or aramid backing. For all further experiments involving firing of ceramic-based inserts, the same backing of 40 layers of Dyneema® SB21 were used. These backing layers meet the requirements for the bulletproof protection level K2 as well as fragment proof protection